PDF (89kB) - Helmholtz-Zentrum Berlin

Fig. 7: Solar cell parameters of TCO/a-Si:H(n)/c-

Si(p) solar cells with variing gas phase doping

concentrations of the a-Si:H layer.

2000 ppm. The open circuit voltage follows the same trend

as the efficiency. Also the short circuit current increases

with increasing NG until NG = 2000 ppm and stays

approximately constant with a further increase of NG. This

result can be interpreted as follows. It is well known that

substitutional doping of a-Si:H on glass substrates leads to

the creation of deep defects. This leads to a self

compensation effect in a-Si:H. However, the maximum

conductivity for P-doped a-Si:H is reported for NG = 10 000

ppm [6] a result that is supported by our findings (Fig. 6).

For amorphous silicon on crystalline silicon the initial

growth of a-Si:H might be different to the case of a-Si:H on

glass substrates. Due to the doping defects are created

which are located at the interface and in the a-Si:H layer.

The optimal gas phase doping concentration is obtained

when the Fermi energy in the a-Si:H layer is sufficiently

close to the conduction band and the defect density is still

considerably low. Obviously the optimum gas phase

doping concentration for a-Si:H/c-Si solar cells is about

2000 ppm.

Using optimized deposition conditions a maximum

efficiency of 17% on a flat c-Si substrate with diffused

back surface field was obtained (Fig. 8). For this

J (mA/cm 2 )

J SC (mA/cm 2 )

V oc (V)

η(%)

0

20

40

32

30

28

0.6

0.5

0.4

12

10

8

(c)

(b)

(a)

0 2000 4000 6000 8000 10000

[SiH ]/[PH ](ppm)

4 3

a-Si:H(n, i)/c-Si(p)/c-Si (p + )

η= 17%

a-Si:H(n)/c-Si(p)/a-Si:H (p + )

η= 17.2%

Fig. 8: Best solar cells using a diffused BSF (c-Si(p + 0.0 -0.2 -0.4

U (V)

-0.6 -0.8

))

and a low temperature a-Si:H(p) BSF.

1228

heterojunction solar cell a thin (3nm) intrinsic amorphous

layer was used. Additionally we fabricated solar cells with

a-Si:H(p) back surface field on a textured substrate but

without special antireflex coating using only low

temperature process steps. Without an intrisic a-Si:H layer

a maximum efficiency of 17.2 % was obtained (see Fig. 8).

This is the highest efficiency of a complete low

temperature a-Si:H(n)/c-Si(p)/a-Si:H(p) solar cell reported

so far.

CONCLUSION

The basic electronic properties of a a-Si:H/c-Si

heterojunction were meaured using PEYS and SPV. The

valence band offset was determined to 0.45 eV.

Simulations show that the interface states density of a a-

Si:H(n)/c-Si(p) has a major impact on the cell efficiency

and must be as low as possible. For the inverse doping

structure Dit plays a minor role. However, with a Dit of

about 2×10 11 cm -2 eV -1 a high efficiency TCO/Si:H(n)/c-Si(p)

cell is achievable. Using optimized deposition conditions

with respect ot the depostion temperature and the gas

phase doping concentration a complete low temperature

processed solar cell with an efficiency above 17 % was

processed.

ACKNOWLEDGEMENTS

This work is supported by the Bundisministerium für

Bildung und Forschung. Contract number FKZ01F0012-19

REFERENCES

[1] M. Tanaka, M. Taguchi, T. Matsuyama, T. Sawada, S.

Tsuda, S. Nakano, H. Hanafusa, Y. Kuwano,

“Development of New a-Si/c-Si Heterojunction Solar

Cells”, Jpn. J. Appl. Phys 31, 1993, p. 3518.

[2] M. Schmidt, A. Schoepke, L. Korte, O. Milch, W. Fuhs,

“The gap state density distribution in extremely thin a-Si:H

layers on crystalline silicon wafers “, J. Non-Cryst. Solids

338-340, 2004, p. 211.

[3] Y. W. Lam, “Surface-state density and surface potential

in MIS capacitors by surface photovoltage

measurements”, J. Phys. D: Appl. Phy.s 4, 1971, p1370.

[4] K. Winer and L. Ley, “Surface states and exponential

valence band tail in a-Si:H”, Phys. Rev. B 36, 1987, p.

6072.

[5] R. Stangl, A. Froitzheim, L. Elstner, M., Schmidt, .

Fuhs, “Amorphous/Crystalline Silicon Heterojunction

Solar Cells, a Simulation Study“, Proc. 17 th EPVSEC,

Munich, 2001, p. 1387.

[6] W. E. Spear and P. G. LeComber , “Substitutional

doping of amorphous silicon”, Solid State Commun. 17,

1975, p.1193.